The wood is dark red brown with purplish shades. The sapwood is clearly demarcated. The grain is straight and the texture is fine. Density at 12 % moisture content: 1.10 g/cm3.
The blunting effect is fairly high; peeling is not recommended or without interest and slicing is reported to be good. Requires power. Nailing is good but pre-boring is necessary. Gluing is correct for interior only. Gluing requires care (very dense wood). It dries slowly and surface drying prior to kiln drying is recommended. Risks of cracks more or less important according to specific gravity.
Massaranduba is very durable to fungi and is durable to dry wood borers; sapwood demarcated (risk limited to sapwood). Due to its high specific gravity and hardness, this species naturally covers the biological hazard class 5 (end-uses in marine environment or in brackish water).
Massaranduba can be used for several applications:
• interior: e.g. sculpture, tool handles, industrial or heavy flooring, sliced veneer, stairs, furniture
• exterior: e.g. ship building, wood frame house, bridges, posts, stakes, sleepers, heavy carpentry
In Brazil, M. elata and M. longifolia are used for pulpwood.
• CIRAD Forestry Department
|Origin:||South and Central America|
Manilkara huberi, Manilkara bidentata,
Macaranduba, Paraju, Nispero, Beefwood, Balata Franc, Balata Rouge, Quinilla Colorada, Balata, Bullet Wood, Maparajuba, Massaranduba, Balata Gomme, Bois Abeille, Pamashto, Bolletrie,
Stakes, Stringed instruments (bow), Hydraulic works (fresh water), Sleepers, Sliced veneer, Ship building (planking and deck), Sculpture, Turned goods, Industrial or heavy flooring, Stairs (inside), Bridges (Parts not in contact with water or ground), Bridges (Parts in contact with water or ground), Poles, Wood frame house, Arched goods, Tool handles (resilient woods), Shingles, Heavy carpentry, Current furniture or furniture components,
|Commercial restriction:||No commercial restriction|
|Typical colour:||Red Brown|
|Crushing strength:||89 (+/- 8) MPa|
|Specific Gravity (at 12% MC):||1,10 (+/- 05) |
|Stability:||Poorly stable |
|Static bending strength:||170 (+/- 18) MPa|
|Strength class:|| |
|Dry wood borers:||Class D - Durable|
|Fungi:||Class 1 - Very durable|
|Termites:||Class D - Durable|
|Treatability:||Class 4 - Not permeable|
Technical descriptions from the software Tropix 7 , with permission of the Research Unit Biomass, Wood, Energy, Bioproducts , CIRAD .
This website is monitored and updated by FSC Denmark. The information displayed is based on the best accessible data and FSC Denmark strives to ensure that all information is correct. FSC Denmark cannot be held responsible for any consequences, such as product failure or other damage arising from the use of information from this website. If any errors or inaccuracies are detected, please contact the web editors through E-mail: